^{1}

^{2}

^{2}

^{1}

The present study aims at helping to search for preventive solutions to pathologies of constructions in Togblécopé in Togo, by the reduction in the withdrawal and swelling of foundation grounds through their stabilization. Togblécopé’s clay taken from 1 m, 2 m and 3 m deep, and mixed with four binding materials (cement, sea sand, silty sand and lime). Tests of identification and free swelling with odometer are carried out on pure and stabilized materials. What emerges from these tests is that the limits of liquidity and plasticity are rising along with the rate of stabilizers while the index of plasticity is falling. Cement and lime cause a reduction in the index value of plasticity by almost 50%. The more the sand’s grain size, the more the reduction in the plasticity index. The swelling potential is reduced by 60% for cement and lime, 30% for sea sand and 20% for silty sand. The present study is a contribution to the reduction in deflations from 20% to 60% of some parts of constructions in order to limit cracks.

Civil engineering works aim at soils called foundation soil that is mostly clayey soils. Some clays present swelling or retracting features. Construction on such a clayey soil requires a thorough campaign of research, identification and characterization of its swelling potential. Swelling soils are very fine soils whose components are made up of layers. The swelling feature is a very complex issue, since it is the outcome of several associated phenomena that cannot be separated in terms of experiment for identification of each mechanism effect [

Therefore, the treatment of soils is often used to upgrade their resistance in order to reduce or to increase their permeability and also to lower their compressibility [

In Togo, or more exactly in Togblécopé, living quarters and other constructions go through sweeping degradations (

- The clay samples are taken from Togblécopé, a suburb located in northern area of Lomé, the capital town of Togo, about 20 km far from the downtown (

The coastal basin (Maastrichtian to Holocene) stretches up to Tsévié and Tabligbo and consequently covers all over this suburb. This basin is composed of sand, clay, limestone and phosphate [

- The CPJ 35 cement manufactured by CIMTOGO and delivered in bags of 50 kg and the lime of the brand CALVIVA, delivered in bags of 25 kg are taken as samples in a commercial store of Lomé in Togo.

- Silty sand and siliceous sand (sea sand) for stabilization, are taken respectively at Dalavé, 35 km in northern area of Lomé on Togo’s littoral in Lomé (

- For different tests the following material is used: manual shaker; mechanical diving shaker with a speed equal to 10,000 tr/mn of the brand MATEST with a vessel; torpedo densimeter with range 0.995 to 1.035; tubes of brand CHEKAMAT and capacity of 2500 ml; consolidation device; oedometric cell of brand S272-01, serial number S272-01/AC/0007; piston of oedometric system; comparator at 1/100 mm; Casagrand device with cup of the brand LABOTEST and serial number Z10248; groover; dryer of the brand Air-Expert with maximal temperature 160˚C; a pycnometer of minimal volume of 500 cm^{3} with roded top; a precision scale of the brand METTLER TOLEDO with a maximal capacity of 5 g and a precision of 0.1 g; a sieve system AFNOR.

The tests are carried out in the laboratory Lab-TP (Laboratory of Public Works) of Lomé in Togo.

Samples of reorganized or intact clayed soil are taken from 1 m, 2 m, and 3 m deep well on the soil of Togblécopé.

The stabilization of the clay from different depths is performed with cement, lime, sea sand and silty sand by proportions of 0% to 10% and at paces of 2% of the material mass.

Physical tests (density, limits of liquidity WL and plasticity WP, equivalent of sand ES and granulometries by sieving and sedimentation) are then carried out on such different materials as clay, sands and on mixtures according to standards [

The free swelling is measured with oedometer on samples subject to the only weight of 1080.22 g of piston (

- Saturation of porous stones for at least 1 hour in a water pit;

- Laying of a porous stone at the base with filter paper;

- Laying of sample of soil cut up in the ring on the basic porous stone;

- Laying of a filter paper on the surface of the sample;

- Laying of the second porous stone and blocking of the whole;

- Positioning of the cell on its plate;

- Filling of the tank with distilled water for the saturation.

The variation of the height of the sample is measured according to the duration of application of the charge (12, 24, 48, 60, 120, 240, 480, 900, 1800, 3600,

7200, 14,400, 21,600, 28,800 in s) until it stabilizes. The sample is considered stable when the difference of reading between two successive times does not exceed 0.001 mm.

The reduction in final swelling Rg(%) is given by:

R g = Δ G G 0 = G 0 − G a G 0 (1)

With Rg the relative reduction in final swelling; G_{o} the reduction in the swelling of pure clay; G_{a} the reduction in the swelling of stabilized clay.

The results of physical tests on the sand and clay materials are given in

- Dalavé’s silty sand has an extended granulometry with a big proportion of sieved sands 0.08 mm of 20.60% with a module of fineness of 1.39 and an equivalent sand of 55. It falls then under the category of very fine sands [

- the sea sand doesn’t contain components that are below 0.160 mm; It has a module of fineness of 2.52 and an equivalent sand of 97.5. This sand is then of medium-sized granulometry [

- the sieved sample sands of 0.08 mm taken at 1 m, 2 m, and 3 m, are respectively of 75.53%, 82.64% and 76.71%. These values are much higher than 50%; the clayed materials from Togblécopé contain then a large proportion of fine grains. Besides, absolute densities of 1 m, 2 m, and 3 m deep can be observed with respectively 2.50, 2.53, 2.54 and indexes of plasticity (Ip) of 25.24,

Materials | Module of fineness | Density | Equivalent de sand (ES in %) | |
---|---|---|---|---|

Apparent | Absolute | |||

Silty sand | 1.39 | 1.59 | 2.61 | 55 |

Sea sand | 2.52 | 1.54 | 2.65 | 95.7 |

34.09 and 41.73. The samples taken at 1 m and 2 m deep can then be considered as plastic whereas those taken at 3 m deep are very plastic. The soils of Togblécopé are therefore more and more plastic and dense in depth than on the surface. This Togblécopé’s soil is an instable land composed of swelling clay.

The results of the average of the limit of liquidity and densities of different composite samples (clays, stabilizers) of different depths are shown in

By examining

- a rise in limits of liquidity and plasticity as the proportion stabilizer increases (

- a reduction in the index value of plasticity while the percentage of stabilizer grows (

- the stabilization with hydraulic binders (lime and cement), presents densities that grow with their dosages; however, densities decrease with the rise in the proportion of sands (

- cement makes clay denser than lime; the density is lower in the case of stabilization with the sea sand than that of silty sand (

- in average 62% of the reduction in the potential of swelling occurs after 30 minutes for the hydraulic binders whereas it is 32% for sands. After 2 hours, 97% of the reduction in swelling occurs for the binders and 89% for the sands. After 8 hours, 100% of the potential of swelling occurs. The equations of levelling of results of proportion of stabilizer of 10%, providing the highest reduction, are shown in (

R g c i m t = 8.717 ln ( t ) − 14.22 and R 2 = 0.921 if t < 4986 (2a)

R g c i m t = 60 if t > 4986 (2b)

R g c h t = 9.832 ln ( t ) − 23.79 and R 2 = 0.935 if t < 5025 (2c)

R g c h t = 60 if t > 5025 (2d)

R g s m t = 4.435 ln ( t ) − 14.41 and R 2 = 0.975 if t < 19200 (2e)

R g s m t = 29.33 if t > 19200 (2f)

R g s s t = 2.877 ln ( t ) − 6.977 and R 2 = 0.958 if t < 11800 (2g)

R g s s t = 20 if t < 11800 (2h)

R_{gcimt}, R_{gcht}, R_{gsmt} and R_{gsst} are respectively reduction in swelling for such additional components as cement, lime, sea sand and silty sand with t the time in s.

- for 10% of stabilizers the four additional components largely reduced the potential of swelling up to 60% for cement and lime, 30% for sea sand and 20% for silty sand (

- The reduction in swelling goes up with the rise in the proportion of stabilizer (

R g c i m T = − 0.883 T 2 + 15.09 T − 2.881 and R 2 = 0.952 (3a)

R g c h T = − 0.837 T 2 + 14.69 T − 3.297 and R 2 = 0.949 (3b)

R g s m T = − 0.125 T 2 + 4.197 T + 0.428 and R 2 = 0.988 (3c)

R g s s T = − 0.180 T 2 + 3.829 T + 0.011 and R 2 = 0.983 (cd)

R_{gcimT}, R_{gchT}, R_{gsmT} and R_{gssT} are respectively reduction in swelling for such additional components as cement, lime, sea sand and silty sand with T the proportion of stabilizer in %.

- for 4% of the proportion of lime and cement, the reduction in swelling is very pronounced; from 8% of all the stabilizers, the reduction in the potential of swelling stabilizes (

- the swelling is more reduced with the hydraulic binders than that of sand; it is also more pronounced for the stabilizer sea sand than that of silty sand (Figures 10-12);

- the potential of reduction in swelling increases with the limits of liquidity and plasticity, it also rises with the index of plasticity (

A reduction in the value of plasticity index when the percentage of stabilizer increases shows that these stabilizers influence the behavior of the clay; which is conform to the works of Djedid who showed that the limits of liquidity and plasticity are key parameters in the swelling behavior of clays [

- the rise in the quantity of pulverilent materials contained in the clayed material that has a plastifying power;

- the formation of a shell wrapping the fine grains of clay material by the minerals (CaO; SiO_{2}; Al_{2}O_{3}) in cement and lime.

The growth of densities of samples from the stabilization at cement and lime according to their mixture proportion (2.498 to 2.578) may be explained by the fact that these two binders make clay more consistent. However, the reduction in the density of samples from the stabilization at sand according to the rise in their proportion and in that the granulometry is high may be justified by the fact that the additional sand makes higher the volume of the mixture whereas the mass goes down.

The rise in the limits of liquidity and plasticity, as the proportion of stabilizer increases, is in line with the results of Cabane [

The reduction in swelling by cement and lime (60%) can be explained the fact that:

- when quick lime and a humid clayed soil are mixed, the quick lime hydrates rapidly by fixing a quantity of water; the divalent cations Ca^{2+} are then able to displace the monovalent cations on the surface of clays [

- on the whole, cement is viewed as a granulometric corrector improving the characteristics of soil. The stabilization of the clay soil with cement forms rapidly calcic hydrates. Thus, the main mineral of cement (CaO; SiO_{2}; Al_{2}O_{3}) builds a shell around the clay as is the case with concretes [

The reduction in the swelling of clay by adding sand is more important when the components of the addition are bigger, showing the effect of the granularity of sand on the swelling (sea sand: 30% and silty sand 20%). This reduction can be interpreted by the fact that the content in clay of the mixtures decreases by addition of sand which is an inert and pulverulent materal. In fact the voids created by the grains of sand in the clay are filled by a large part the swelling [

The significant reduction in the Togblécopé’s clay by different techniques of stabilization helps contribute to the preventions of works’ pathologies, since this swelling soil causes a degree of growing saturation by capillarity under the buildings whereas the direct periphery remains subject to seasoning climate variations. This phenomenon causes differential movements of parts of the buildings leading to their excessive distortions. Thus, the reduction in the potential of swelling leads to the reduction in differential movements of some parts of the buildings. This results in the reduction in the excessive distortions in these parts.

The study showed that it is possible, considering cement, lime and sands as stabilizers, to reduce the swellingpotential of Togblecopéswellingsoils in Togo. The buildings undergoing excessive deformations due to swelling of the foundation soil of the zone, this reduction of swelling will thus allow the attenuation of the differential movements of the parts of the buildings thus reducing the appearance of the cracks. For the rest of this work, a study must be made through tests of determination of the mechanical strengths in order to appreciate the mechanical behavior of this swelling sol with respect to the stabilization.

This work could not have been carried out without the logistic and financial support from FORMATEC we express our sincere gratitude to.

Amey, K.B., Sounsah, K.M., Amoussou, K.A.S. and Neglo, K. (2018) The Reduction in the Swelling Potential of the Foundation Ground of Togblécopé in Togo by the Stabilization with Binders and Sands. Open Journal of Civil Engineering, 8, 221-233. https://doi.org/10.4236/ojce.2018.82017